HAL Id: hal-01322252
Submitted on 26 Sep 2017
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Fatigue resistance of natural rubber in seawater with
comparison to air
Kubat Narynbek Ulu, Bertrand Huneau, Pierre-Yves Le Gac, Erwan Verron
To cite this version:
Kubat Narynbek Ulu, Bertrand Huneau, Pierre-Yves Le Gac, Erwan Verron. Fatigue resistance of
natural rubber in seawater with comparison to air. International Journal of Fatigue, Elsevier, 2016,
88, pp.247-256. �10.1016/j.ijfatigue.2016.03.033�. �hal-01322252�
Fatigue resistance of natural rubber in seawater with comparison to air
K. Narynbek Ulua,b,1
, B. Huneaua,⇑
, P.-Y. Le Gacb
, E. Verrona
Ecole Centrale de Nantes, Institut de Recherche en Génie Civil et Mécanique (GeM), UMR CNRS 6183, Nantes, France
IFREMER, Centre de Bretagne, Marine Structures Laboratory, Brest, France
Keywords: Natural rubber Fatigue Environmental effects Seawater Strain-induced crystallization Fatigue properties of filled natural rubber in seawater environment are investigated by uniaxial fatigue
and crack propagation experiments, and the damage is analyzed by scanning electron microscopy. The behavior under relaxing and non-relaxing loading conditions is studied and the results are compared to those obtained in air environment. For relaxing loading conditions, fatigue behavior is the same in both environments. Under non-relaxing conditions at large strain levels, for which the influence of strain-induced crystallization is important, fatigue life is longer in seawater. Such behavior could be explained by increased internal temperatures of specimens tested in air due to lower heat conductivity of air as compared to seawater. Such conclusion is also supported by the damage mechanisms observed under non-relaxing loading conditions.
Natural rubber (NR) is a versatile elastomer that has been used industrially for well over a century. It has found use in many differ-ent applications mainly because of its ability to dissipate energy and undergo large elastic deformation whilst maintaining excellent resistance to crack growth. The majority of NR is used in production of automobile tires. Additionally, it finds use in the marine environ-ment (upon a selection of appropriate formulations) because of its low water absorption and consistent mechanical properties after prolonged immersion in seawater. With recent growth of interest in off-shore energy production, ranging from oil or natural gas, wave, wind to tidal energy, better understanding of fatigue behavior of natural rubber in seawater is of interest at present.
The study of NR fatigue is divided into two complementary approaches that lead to determination of fatigue life: the crack nucleation approach, which focuses on the prediction of crack ini-tiation in a material without defects; and, the crack propagation approach, which considers the cyclic growth of an existing crack. The crack nucleation approach refers to continuum mechanics, whereas the crack propagation approach refers to fracture mechanics. Several factors influence fatigue properties of NR. In general, they are separated into three groups: mechanical load-ing conditions, environmental conditions, and chemical
formula-tion (addiformula-tion of antioxidants, antiozonants, fillers, and other additives used in the industrial process).
The mechanical loading conditions for soft materials are usually defined by prescribed displacement or strain energy density. In both cases, we classically define the R-ratio, or the loading ratio, as the ratio of the minimum to the maximum loading quantity. In terms of the stretch ratiok ¼ l=l0, it is defined as:
ðkmax 1Þ ð1Þ
The R-ratio is a useful descriptor of mechanical loading and its value considerably affects the fatigue behavior. For R = 0, i.e. the mini-mum loading quantity is zero, the mechanical loading conditions are said to be relaxing; when R > 0, i.e. the minimum loading quan-tity is positive, they are said to be non-relaxing. Under the latter type of loading conditions, fatigue resistance of NR improves (nota-bly in contrast to metals). The general consensus is that presence of strain-induced crystallization (SIC) is responsible for such improve-ment[4,5]. The effects of SIC in fatigue will be discussed in further detail in Section 4. For further information on SIC in rubber, the reader can refer to the review articles of Tosakaand Huneau. The second factor that influences fatigue properties of rubber is the environment. In air, the fatigue behavior has been extensively studied: see for example Cadwell et al., Rivlin and Thomas, Lindley [4,10], Lake , and many others. In air, fatigue is a mechanico-oxidative process. Comparison with results in an oxygen free environment (nitrogen) reveals that gaseous oxygen accelerates crack growth and decreases the fatigue crack propaga-tion threshold. A study by Gent and Hindishows that in ⇑ Corresponding author at: Ecole Centrale de Nantes, 1 Rue de la Noë, 44321
E-mail address:firstname.lastname@example.org(B. Huneau).
vacuum environment, i.e. with no exposure to oxygen, the crack propagation rate is reduced roughly by a factor of 2 as compared to air environment. Oxygen also has a long term effect on NR fati-gue due to aging, which is driven by diffusion of oxygen in NR; pri-marily, it affects the mechanical properties making it hard and brittle . For NR, aging reduces the fatigue life, fastens crack propagation, and reduces fatigue threshold.
In contrast, effects of seawater (or water in general) on NR fati-gue have not been investigated to the same extent as in air. Mott and Roland  carried out accelerated aging experiments and found that the concentration of oxygen in seawater has a direct effect on degradation of NR. As for fatigue behavior, under relaxing loading conditions (R = 0), one study suggests that fatigue crack propagation rates are almost identical to the ones in air. More-over, after a long-term immersion in seawater of 2.25 years, no dif-ference (compared to air) in crack propagation properties has been observed for R = 0. Additionally, it has been shown that fatigue life under relaxing loading conditions is similar in distilled water
and in seawateras compared to air. On the other hand, under non-relaxing loading conditions at R = 0.2, the fatigue threshold is higher and crack propagation is slower in water com-pared to air regardless of temperature. In the recent study of Le Gac et al., a decrease in fatigue life is observed in seawater compared to air under non-relaxing loading conditions; this result is obtained for filled NR (15 phr of carbon black) with and without antioxidants. Moreover, it appears that antioxidant leaching has no effect on fatigue life of NR in seawater.
In the present paper, the focus is primarily on mechanical load-ing and environment. Since fatigue properties of NR are relatively well-understood in air, the objective is to compare these properties in seawater; an important question is whether the vast knowledge of fatigue behavior in air can be expanded to the seawater environ-ment. The present work parallels the study of Le Gac et al., specifically, to a greater range of strain levels under which the ben-eficial effects of strain-induced crystallization are greatly enhanced. Both fatigue life and fatigue crack propagation experi-ments are carried out, and the corresponding damage mechanisms are observed by scanning electron microscopy (SEM).
2. Experimental program
The composition of the studied material is given inTable 1. The material is molded into sheets of 2 mm uniform thickness and the specimens are cut using a die and a pneumatic press. The experi-ments are performed on a virgin material and no pre-aging steps are considered.
Fatigue life tests are performed on flat dumbbell specimens (H3) with dimensions shown in Fig. 1 (ISO 37:2005 standard, dumbbell: type 3). In the middle of the specimen, the gauge length is 17 mm long and the stress state is that of uniaxial tension. Fati-gue crack propagation tests are performed on single-edge-notched tension (SENT) specimens shown in Fig. 2; the dimensions are 146 mm 25 mm 2 mm and a 1 mm cut is introduced in the middle of the specimen with a brand new blade. The design of the experimental grips reduces the effective length of H3 and SENT specimens to 28 mm and 96 mm respectively.
2.3. Experimental procedure
Actual fatigue tests are performed on custom-built electrically driven machines (actuators Parker PRA 3810S). The testing machi-nes apply a sinusoidal waveform that is displacement controlled. The sinusoidal movement of the actuators is verified manually (minimum and maximum positions) and by using an LVDT. Tests are performed in both air and seawater environments. The loading ratios R = 0 and R = 0.2 are considered. These values are calculated considering the local maximum stretch ratio klocal. All fatigue experiments are performed at 2.0 Hz. Experiments in air are car-ried out at laboratory room temperature, i.e. 22°C. For the experi-ments in seawater, specimens are submerged into home-made tanks (12 L in volume). The seawater is extracted directly from the roadstead of Brest and its properties are shown inTable 2. Seawater is continuously renewed by slow drainage and addition of extra seawater; the rate of water flow through the tank is in the order of magnitude of 1 L/h, which does not affect the temper-ature that is held constant at 25°C by using a thermocouple-controlled heater. Water is aerated and its closed circulation is managed by a pump. The seawater is replaced for each test. The experimental setup for fatigue life tests is shown inFig. 3.
Before the fatigue experiments, the Mullins effect is removed by performing 50 cycles at 110% of the maximum local stretch ratio prescribed in fatigue experiments. The frequency of these accom-modation cycles is set to 0.5 Hz and a 15 min long relaxation per-iod is imposed between accommodation and start of the fatigue experiments.
2.3.1. Preliminary tests
The maximum local stretch ratio klocal differs from the pre-scribed global stretch ratio due to sample geometry. Here, the local stretch ratio is measured by digital image correlation (DIC). The material stress–strain response and the details of the DIC experi-ments are expanded in Appendix A. Additionally, experiments Nomenclature
6PPD N-[1,3-Dimethylbutyl]-N0-phenyl-p-phenylenediamine (antioxidant, antiozonant)
c crack length of a SENT specimen CB carbon black
CBS N-cyclohexyl-2-benzothiazolesulphenamide (vulcaniza-tion accelerator)
k constant as a function of maximum stretch ratio relating tearing energy to strain energy density for SENT speci-men
l deformed length l0 initial length
EDS energy dispersive spectroscopy LVDT linear variable differential transformer NR natural rubber
SENT single-edge notched tension specimen SEM scanning electron microscopy SIC strain-induced crystallization R loading ratio
T tearing energy W strain energy density k global stretch ratio
Dk amplitude based on maximum local stretch ratio klocal maximum local stretch ratio within the specimen
kmax maximum amplitude based on maximum local stretch
kmin minimum amplitude based on maximum local stretch
are carried out to measure the heat build-up of the H3 specimens in air. The average temperatures of the surface of the specimen are monitored using an infrared thermometer for given maximum stretch ratiosklocal= 1.5, 2.0, 2.5, 3.0 and 4.15 at a frequency of 2 Hz. 2.3.2. Fatigue life
For fatigue life experiments, the end-of-life criterion is defined as the number of cycles until complete failure of the specimen. Experiments are carried out at constant stretch ratio amplitudes
Dk = kmax kmin= 1.0, 1.5, 2.0, and 2.5, for R = 0 and R = 0.2; values for maximum and minimum applied stretch ratios are shown in
Table 3. The corresponding displacements prescribed to the testing machines are calculated from the DIC results. Special home-made grips allowed to test up to 7 specimens per single experiment. With fatigue life testing of rubbers in general, there is usually a high dispersion of results due to presence of preexisting micro-scopic flaws of inhomogeneous sizes[20,21]. Therefore, for statis-tical significance, at least 14 specimens are tested for each loading level at R = 0 and R = 0.2 in each environment.
2.3.3. Fatigue crack propagation
Crack propagation experiments are performed at low and high stretch ratio amplitudes in order to measure crack growth rates for a wide range of tearing energies. Due to testing machine con-straints, the prescribed amplitudes vary fromDk = 0.3 toDk = 0.7 for both loading ratios; values for maximum and minimum applied stretch ratios are shown inTable 4. The tearing energy of the SENT specimen is approximately related to the crack length c and the strain energy density W by:
T¼ 2kWc ð2Þ
p=pﬃﬃﬃk. The value of W is measured experimentally as the total area under the stress–strain curve after accommodation cycles. Experiments are run continuously at constant amplitudes
until fracture of the specimen and the crack length is recorded by a high speed camera. However, during experiments under R = 0.2, crack branching occurs where secondary cracks are formed and their growth direction is not perpendicular to the loading direction. In such cases, a test is stopped if crack branching occurs for crack lengths greater than half of the width of the SENT specimen; if crack branching occurs for crack lengths less than half of the width of the specimen, the test is paused and a new notch is cut along the orig-inal path of the crack in the direction perpendicular to the direction of loading. Crack propagation rate measurements are made only after the fatigue blunting of the new notch.
2.3.4. Damage mechanism analysis
JEOL JSM-6060LA scanning electron microscope (SEM) is used for microscopic analysis of specimens tested for fatigue life. The fractured specimens and those obtained from interrupted tests just before failure are considered; the interrupted tests are carried out at stretch amplitudeDk = 1.5 and R = 0.2 in both air and seawater. All specimens are stretched up to k = 1.3 using a Deben
micro-Table 1 Material composition. Ingredients Amount (phr) Natural rubber 100 Carbon black 45 Sulfur 1.5 CBS 1.5 Stearic acid 2.0 Zinc oxide 2.5 6PPD 2.0
Fig. 1. Dimensions of H3 specimen used for fatigue life tests.
Fig. 2. Dimensions of SENT specimen used for crack propagation tests.
Properties of seawater extracted from the roadstead of Brest (data provided by SOMLIThttp://somlit-db.epoc.u-bordeaux1.fr/bdd.php). Min Max Experimental temperature (°C) 25.00 Salinity (PSU) 34.40 35.13 Oxygen content (mL/L) 5.44 6.47 pH 7.96 8.11
tensile machine in order to open cracks and defects during obser-vations. Additionally, energy dispersive spectroscopy (EDS) is used to inspect the chemical composition of surfaces around and within the cracks by keeping the electron beam stationary on several points for localized information.
3.1. Fatigue life
The fatigue life results are shown on a Wöhler curve, where the fatigue life (number of cycles to failure) in both environments is plotted with respect to the stretch amplitudeDk (Fig. 4). The geo-metric averages of fatigue lives with their 95% confidence intervals are presented for each testing condition. The equation for calcula-tion of 95% confidence intervals is the following:
C95¼ t95 s p
where s is the estimated standard deviation, n is the number of tested specimens, and t95 is the upper (1 0.95)/2 critical value for a T-Distribution (since the true standard deviation is not known) with n 1 degrees of freedom. Because testing of 14 specimens for each testing condition in each environment provides statistical sig-nificance, small differences in the fatigue life results can be discussed.
In general, the fatigue life decreases as stretch ratio amplitude increases for both relaxing (R = 0) and non-relaxing (R = 0.2) load-ing conditions. The average fatigue lives and the correspondload-ing 95% confidence intervals in seawater and in air significantly over-lap under relaxing loading conditions (R = 0). For all loading levels, it is clear that the fatigue lives are identical in both environments. As expected, under non-relaxing loading conditions (R = 0.2), the fatigue life increases in both environments. Moreover, the aver-age fatigue life atDk = 0.5 decreases by around 7% in seawater as compared to air with a considerable overlap of the confidence intervals. AtDk = 1.0, the average fatigue life in seawater decreases by around 21% as compared to air within the boundaries of confi-dence intervals. The average fatigue life atDk = 1.5 in seawater increases by around 6%, but also with a considerable overlap of the confidence intervals. Finally, the fatigue life in seawater is revealed to be longer than in air for large stretch ratio amplitudes (an increase of around 66% atDk = 2.0 and 77% atDk = 2.5). 3.2. Fatigue crack propagation
The fatigue crack propagation results are shown inFig. 5, where the crack propagation rate is plotted with respect to the tearing energy. The crack propagation rate is identical in seawater and air under both loading conditions, R = 0 and R = 0.2. Moreover, the crack propagation rate under non-relaxing loading conditions is slower and the fatigue threshold increases in both seawater and air in comparison to relaxing loading conditions. It should be noted that crack branching is observed during experiments under non-relaxing loading conditions (Fig. 6).
3.3. Damage mechanism analysis
Surfaces of specimens tested for fatigue life are inspected using scanning electron microscopy (SEM) (Figs. 7–12). Microscopic
Fig. 3. Experimental setup for fatigue life tests in seawater (for experiments in air, the tests are performed on the same setup but without water); magnified is the design of the grips.
Maximum and minimum applied stretch ratios for each fatigue life test level. Level/ amplitude R = 0 R = 0.2 Min. local stretch Max. local stretch Min. local stretch Max. local stretch 1:ka= 0.50 1 1.50 1.13 1.63 2:ka= 1.00 1 2.00 1.25 2.25 3:ka= 1.50 1 2.50 1.38 2.88 4:ka= 2.00 1 3.00 1.51 3.51 5:ka= 2.50 1 3.50 1.65 4.15 Table 4
Maximum and minimum applied stretch ratios for each crack propagation test level.
Level/ amplitude R = 0 R = 0.2 Min. local stretch Max. local stretch Min. local stretch Max. local stretch 1:ka= 0.10 1 1.10 1.03 1.13 2:ka= 0.20 1 1.20 1.05 1.25 3:ka= 0.30 1 1.30 1.07 1.37 4:ka= 0.40 1 1.40 1.10 1.50 5:ka= 0.50 1 1.50 1.12 1.62 6:ka= 0.60 1 1.60 1.15 1.75 7:ka= 0.70 1 1.70 N/A N/A
damage features are similar irrespective of the stretch ratio ampli-tude and the environment for relaxing loading conditions R = 0 (Fig. 7). Cracks form on a plane perpendicular to the loading direc-tion and their lengths vary from 100
lm to 500
lm. Crack densities on the surface increase with stretch ratio amplitude in a similar manner for both environments.
Under non-relaxing loading conditions (R = 0.2), morphology of cracks differs between air and seawater. In air, cracks appear on a
plane perpendicular to the loading direction (Fig. 8a). Damage in seawater is completely different. Cracks appear in form of a cross on the surface and two cones form an ‘‘hourglass-shape” in 3D; qualitatively speaking, the majority of such cracks are symmetric
1 000 000.00
10 000 000.00
Stretch Rao Amplitude,
Fague Life (Cycles)
Fig. 4. Fatigue life of NR in seawater and air at R = 0 and R = 0.2.
0.000001 0.00001 0.0001 0.001 0.01 1 10 100
Crack Propagaon Rate, dc/dN, mm/cycle
Tearing Energy, T, kN/m
R=0, Air R=0.2 Air R=0, Seawater R=0.2, Seawater Fig. 5. Fatigue crack propagation rate of NR in seawater and air at R = 0 and R = 0.2.
Fig. 6. Example of crack branching under R = 0.2 loading of a SENT specimen (direction of loading is vertical).
with only few cracks appearing in form of a half of an ‘‘hourglass.” Energy dispersive spectroscopy does not identify in the matrix any foreign inclusions such as oxides or other poorly dispersed com-pound ingredients within cracks. The difference in the damage mechanisms is also revealed by edge cracks. In seawater, the direc-tion of crack growth is parallel to the loading direcdirec-tion, and both crack branching and secondary cracks are observed (Fig. 9b). How-ever in air, the cracks are mostly uniform and develop on a plane perpendicular to the loading direction (Fig. 9a). Moreover, a high density of microscopic cracks (inferior to 100
lm in length) is observed on specimens tested in air (Fig. 10), but similar features do not take place in seawater.
Additionally, the effect of the stretch amplitude under non-relaxing loading conditions is shown inFigs. 11 and 12. The crack morphology depends on both the stretch ratio amplitude and the environment. In seawater, crack paths on the surface evolve from smooth curves at lower stretch ratio amplitudes (Fig. 11a) to more irregular ones at higher ones (Fig. 11b). In air, the crack morphol-ogy is similar for low (Fig. 12a) and high (Fig. 12b) amplitudes with only difference in their densities: the number of cracks of all sizes increases as the stretch ratio amplitude increases.
4.1. Relaxing loading conditions
Under relaxing loading conditions (R = 0), the three experimen-tal approaches reveal with significant correlation that the fatigue behavior of NR is similar in seawater and in air. Primarily, fatigue
lives are the same in both environments for all stretch ratio ampli-tudes. These results agree with those of Le Gac et al.. Secondly, the crack propagation behavior is also identical in both environ-ments; likewise, this is in agreement with literature. Thirdly, the damage mechanisms observed by SEM are the same in both environments; cracks in seawater and air are perpendicular to the direction of loading. Thus, it appears that NR fatigue properties under relaxing loading conditions are not affected in a positive or negative manner by seawater in comparison to the properties in air.
4.2. Non-relaxing loading conditions
On the other hand, the results under non-relaxing conditions (R = 0.2) are not as clear-cut. The results highlight a considerable improvement of fatigue lives and reduction of crack growth rates at R = 0.2 in comparison to R = 0 loading conditions for both air and seawater. Therefore, it is sensible to first discuss the overall effect of the R-ratio separately from the effect of the environment.
4.2.1. Effect of positive R-ratio irrespective of the environment As mentioned in the introduction, it is widely accepted that improved fatigue properties of NR for R > 0 are due to increased presence of SIC in NR. It is now well-established that under quasi-static loading conditions, strain-induced crystallites appear at a given threshold stretch ratio (for 50 phr carbon black content,
Fig. 7. SEM micrographs in (a) air and (b) seawater under relaxing loading
conditions; horizontal direction of loading; failed specimen stretched atDk = 1.5. Fig. 8. SEM micrographs in (a) air and (b) seawater under non-relaxing loading conditions; horizontal direction of loading; interrupted specimen right before failure stretched atDk = 1.5.
it varies from around 2.0 to 2.4); moreover during unloading, the crystallites melt at a smaller threshold stretch ratio, which for filled NR is close to the above-mentioned crystallization stretch ratio [22–24]. It should be noted that these threshold values change with both temperature and strain rate. Thus, no pre-cise values of these quantities will be given in the following discus-sion. As a consequence, the influence of SIC on fatigue properties depends on both minimum and maximum cyclic stretch ratios,
and thus on the R-ratio: number of studies have demonstrated that fatigue life increases as R-ratio increases[8,27,28]mainly because fatigue crack growth is retarded[4,13,20,29,30]. This hypothesis is supported by the results of crack propagation experiments. In ini-tial observations, there is the occurrence of crack branching due to SIC under non-relaxing loading conditions. Since the crystalline regions at the crack tip are significantly larger and induce an aniso-tropic microstructure[34,29,30], the symmetry around the crack disappears and the crack branches out with growth proceeding in a path not perpendicular to the direction of loading. This obser-vation is reinforced by the experimental results, where the crack propagation rate is slower and the fatigue threshold is generally higher for R = 0.2 as compared to R = 0.
However, the positive effect of non-relaxing loading conditions differs in regards to the stretch ratio amplitude. For R = 0.2 loading, the relative increase of fatigue life observed between the results for
Dk = 1.0 and those for Dk = 0.5 (with respective maximum stretches ofkmax= 2.25 andkmax= 1.63) is almost negligible consid-ering the large decrease in the stretching level. The incidence of SIC and its beneficial effects are reduced forDk = 0.5 in comparison to
Dk = 1.0; it can be explained by the relative position of the loading conditions with respect to the above-mentioned crystallization and melting thresholds[23,31].
For higher stretch ratio amplitudes (Dk P 1.5), there are how-ever three competing phenomena. First, the material reinforces due to the increase in crystallinity during cyclic loading. Neverthe-less, it is counteracted by the effect of large loading, which pro-motes damage and therefore shortens fatigue life. The third phenomenon is the increase of heat build-up due to high stretch
Fig. 9. SEM micrographs of edges in (a) air and (b) seawater under non-relaxing loading conditions; horizontal direction of loading; interrupted specimen right before failure loaded atDk = 1.5.
Fig. 10. Small cracks on the surface of a specimen tested in air at R = 0.2; horizontal direction of loading; failed specimen loaded atDk = 0.5.
Fig. 11. SEM micrographs in seawater under non-relaxing loading conditions at (a) Dk = 1.0 and (b) Dk = 2.0; horizontal direction of loading; taken at failure.
ratio amplitudes, which also greatly contributes to deterioration in fatigue properties[32,13]. These three factors explain why the pos-itive effect of R-ratio on fatigue life diminishes with increasing strain levels forDk P 1.5.
4.2.2. Effect of the seawater environment in comparison to air Due to these different behaviors at low and large stretch ratio amplitudes, the effect of seawater on fatigue properties under non-relaxing loading conditions is now discussed in the two next sections.
22.214.171.124. Low stretch ratio amplitudes. ForDk = 0.5, 1.0 and 1.5, fati-gue lives in seawater and air are close and within the 95% confi-dence intervals. Although, the experimental methods of the present work differ to those of Le Gac et al., a comparison of the results can be performed. Loading conditions considered in Le Gac et al. parallel the low stretch ratio amplitudes investigated in the present work (Fig. 13). At first glance, the results of Le Gac et al. and of the present work could appear different: Le Gac et al. observe a tangible difference in fatigue life in both environ-ments. However, some parallels are noticeable upon closer inspec-tion of the present results. The average fatigue lives are shorter in seawater than in air within the stretch ratio amplitude range
Dk = 0.5–1.0: the difference in fatigue life is about 7% with a signif-icant 98% overlap of the confidence intervals forDk = 0.5 and, for
Dk = 1.0, it is about 26% with a 22% overlap of the confidence inter-vals. However, in the present work, the fatigue lives (in both air and seawater) are longer. These discrepancies between the two studies are explained by different experimental methods: most
importantly, the material formulations are different. The longer fatigue lives of the present work can be explained because the pre-sent material has a higher CB content (45 phr vs 15 phr). With ref-erence to the earlier discussion in Section4.2.1, the stretch ratio thresholds at which crystallization appears and melts depends on filler content; these thresholds are higher for NR with carbon black content of 15% as compared to 45%[22,25,24]. As such, the benefi-cial influence of SIC is greater in the present work under the effects of non-relaxing loading conditions.
Now, considering that the fatigue crack propagation is the same in both environments, it suggests that crack nucleation and subse-quent growth occur slightly earlier in seawater for low stretch ratio amplitudes. It is difficult to give a precise explanation for this phe-nomenon. Le Gac et al. suggest that the decrease in fatigue life could be attributed to reduced presence of SIC in seawater. Another explanation can be proposed: the influence of air (oxygen) on the formation of multiple micro-cracks on the surface of the specimens as shown inFig. 10; these micro-cracks appear at all stretch ratio amplitudes on specimens tested in air, but are absent on those tested in seawater. We argue that the energy available for crack growth is distributed amongst all these micro-cracks, thus retard-ing the emergence of a main crack which causes the failure. Obvi-ously, this phenomenon should not be taken into account at the very end of fatigue life when crack coalescence takes place.
126.96.36.199. Large stretch ratio amplitudes. For stretch ratio amplitudes
Dk = 2.0 and 2.5, fatigue lives are longer in seawater than in air (these amplitudes are larger than those considered in Le Gac et al.). Compared to the low stretch ratio amplitudes, the principal differences are: a higher incidence of SIC due to the increase in the minimum stretch ratiokmin; and higher specimen temperatures in air than in seawater due to heat build-up of NR. Indeed, as men-tioned above, seawater temperature is held constant at 25°C; thus, it can be argued that the surface temperatures of seawater tested specimens are in equilibrium around this temperature because of high heat conductivity of seawater. Conversely, air is a much poorer conductor of heat (lower by a factor of about 30 as com-pared to seawater) and therefore, for the largest stretch ratio amplitude the surface temperature in air is measured to be about 35°C. As noted previously, the fatigue life shortens and crack prop-agation rates increase at elevated temperatures. This argument does not contradict fatigue crack propagation results. Indeed, the temperature of SENT specimens in air is not as large as the one in H3 because of a smaller prescribed stretch ratio and a larger sur-face area of the SENT specimens; thus crack propagation results are the same in both environments and they do not correlate to the fatigue life tests measured for large stretch ratio amplitudes.
Addi-Fig. 12. SEM micrographs in air under non-relaxing loading conditions at (a) Dk = 1.0 and (b) Dk = 2.0; horizontal direction of loading; taken at failure.
0 0.5 1 1.5 2 2.5 3 10000 100000 1000000 10000000
Stretch Rao Amplitude,
Fague Life (Cycles)
R=0.2, Air R=0.2, SEAWATER LeGac2014: R=0.2, Air LeGac2014: R=0.2, SW
Fig. 13. R = 0.2 fatigue life results in seawater and air compared to the results of Le Gac et al..
tionally, the incidence of SIC in NR highly depends on temperature: as it increases, the onset of crystallization is shifted toward higher values ofk and the total levels of crystallinity decrease. To confirm the hypothesis of the deleterious effect of heat build-up in air, supplementary fatigue life experiments are carried out for these large stretch ratio amplitudes, under the same testing condi-tions, and in both environments at a lower frequency of 0.5 Hz. This reduces the temperature in air-tested specimens; however, the temperature of the water-tested specimens remains around 25°C (the temperature of seawater) because of higher heat con-ductivity. The hypothesis is confirmed with the fatigue life being the same in both environments. With these explanations, it is pos-sible to rationalize the longer fatigue life in seawater as compared to the one in air for large stretch ratio amplitudes.
In regards to scanning electron microscopy, the damage observed in air under non-relaxing loading conditions is typical to that of oxygen/ozone aging, where numerous cracks are present and are perpendicular to the direction of loading (Fig. 8a). In con-trast, the damage in seawater is noticeably different (Fig. 8b); these observations are original and have not been encountered in litera-ture. More so, the mechanisms behind this type of damage are unknown. It should be noted that no inclusions have been detected by EDS and, as such, do not appear to be responsible for the initi-ation of the cracks. At first glance, if one considers only one half of the symmetric ‘‘hourglass” cracks, it could appear to resemble decohesion at the poles due to presence of CB agglomerates. Consequently, the presence of symmetry would imply formation of cracks in exact pairs, i.e. initiation of these cracks due to a pair of CB agglomerates, which is highly unlikely. Moreover, conical shaped crack induced by CB agglomerates has not been reported in the literature. Therefore, initiation due to carbon black agglom-erates can also be excluded.
In seawater, the morphology of edge cracks is indicative of the effects of SIC (Fig. 9b), where the cracks propagate in the direction parallel to the direction of loading. This is analogous to the crack branching phenomenon observed during fatigue crack propagation experiments under non-relaxing conditions. Additionally, the increased irregularity of crack paths at larger stretch ratio amplitudes in seawater is also characteristic of crack branching and, accordingly, is indicative of a large presence of local crystallinity (Fig. 11b). The absence of such branching at larger stretch ratio amplitudes in air supports the hypothesis that the incidence of SIC is reduced under high internal temperatures of the specimens (Fig. 12).
Three experimental techniques are applied to study the fatigue properties of NR in seawater under both relaxing and non-relaxing loading conditions: fatigue life and crack propagation experiments, and SEM analysis. Results show that the NR fatigue properties in
seawater are identical to that in air under relaxing loading condi-tions (R = 0). For non-relaxing loading condicondi-tions (R = 0.2), where increased beneficial effects of strain-induced crystallization are observed, the fatigue behavior in seawater differs from that in air. At small stretch ratio amplitudes (Dk = 0.5, 1.0, 1.5), the fatigue life is very close in seawater and in air. However, the fatigue life is longer in seawater than in air for large stretch ratio amplitudes (Dk = 2.0 and 2.5). Heat build-up of specimens at large stretch ratio amplitudes appears to have significant influence on the properties: because of thermal properties of seawater, temperatures of speci-mens in seawater are lower than temperatures of the ones tested in air. Degradation of fatigue properties at high temperatures could be attributed to the reduction of the beneficial effects of SIC in such conditions. This conclusion is supported by the damage observed in seawater and air for R = 0.2 loading conditions. The damage mechanisms in seawater appear to be unique and are not fully understood. However, increased presence of crack branching in seawater and its relative absence in air points to reduction of SIC in specimens tested in air for large stretch ratio amplitudes and high temperatures.
The authors would like to thank P. Guégan and F. Pasco of Ecole Centrale de Nantes, and M. Premel-Cabic of Ifremer for their assis-tance during experimental campaigns.
The contents of Appendix A are related to the uniaxial mechan-ical behavior of the present material as obtained from tensile tests
0 5 10 15 20 25 30 1 2 3 4 5 6 Nominal stress (M Pa)
Local stretch rao
Fig. A.1. Uniaxial stress–strain behavior of the tested material.
1 1.5 2 2.5 3 3.5 4 1 1.5 2 2.5 3 3.5 4 Gl obal Stretch Rao, λgl obal
Max. Local Stretch Rao, λmax
1 1.25 1.5 1.75 2 1 1.25 1.5 1.75 2 Gl obal Stretch Rao, λgl obal
Max. Local Stretch Rao, λmax
and digital image correlation (DIC). Before tensile testing, the spec-imens are preconditioned for 50 cycles.
The stress–strain experimental data are shown inFig. A.1. Digital image correlation is used to find the relationship between the global and the maximum local stretch ratios. Com-mercial software Vic2D is used to measure the local stretch ratio; after calibration, the software automatically calculates the Hencky strain on a speckled specimen. The magnitude of the Hencky strain is related to the local stretch ratio by the following equation:
¼ lnðkÞ ðA:1Þ
The results of DIC analysis show a linear correlation between local and global stretch ratios for both H3 and SENT specimens (Fig. A.2).
Mars W, Fatemi A. A literature survey on fatigue analysis approaches for rubber. Int J Fatigue 2002;24:949–61.
Mars W. Factors that affect the fatigue life of rubber: a literature survey. Rubber Chem Technol 2004;77:391–412.
Beatty J. Fatigue of rubber. Rubber Chem Technol 1964;37(5):1341–64. Lindley PB. Relation between hysteresis and the dynamic crack growth
resistance of natural rubber. Int J Fract 1973;9(4):449–62.
Gent AN, Zhang L-Q. Strain-induced crystallization and strength of rubber. Rubber Chem Technol 2002;75(5):923–33.
Tosaka M. Strain-induced crystallization of crosslinked natural rubber as revealed by X-ray diffraction using synchrotron radiation. Polym J 2007;39:1207–20.
Huneau B. Strain-induced crystallization of natural rubber: a review of X-ray diffraction investigations. Rubber Chem Technol 2011;84(3):425–52. Cadwell S, Merrill R, Sloman C, Yost F. Fatigue life of rubber. Ind Eng Chem Anal
Rivlin R, Thomas A. Rupture of rubber. I. Characteristic energy for tearing. J Polym Sci 1953;10(3):291–318.
Lindley PB. Energy for crack growth in model rubber components. J Strain Anal 1972;7:132–40.
Lake G. Fatigue and fracture of elastomers. Rubber Chem Technol 1995;68:435–60.
Lake G, Lindley PB. The mechanical fatigue limit for rubber. J Appl Polym Sci 1965;9:1233–51.
Legorju-Jago K, Bathias C. Fatigue initiation and propagation in natural and synthetic rubbers. Int J Fatigue 2002;24:85–92.
Gent A, Hindi M. Effect of oxygen on the tear strength of elastomers. Rubber Chem Technol 1990;63:123–34.
Datta R, Huntink N. Rubber vulcanizates degradation and stabilization. Rubber Chem Technol 2000;80:435–80.
Mott PH, Roland CM. Aging of natural rubber in air and seawater. Rubber Chem Technol 2001;74(1):79–88.
Selden R. The effect of water immersion on fatigue crack growth of two engineering rubbers. J Appl Polym Sci 1998;69:941–6.
Lake G, Pond T. Effects of aqueous environments on fatigue and elastic properties of rubber. Polym Mar Environ 1989:141–7.
Le Gac P, Arhant M, Davies P, Muhr A. Fatigue behaviour of natural rubber in marine environment: comparison between air and seawater. Mater Des 2014;65:462–7.
Mars W, Fatemi A. Fatigue crack nucleation and growth in filled natural rubber. Fatigue Fract Eng Mater Struct 2003;26:779–89.
Li F, Liu J, Mars W, Chan T, Lu Y, Yang H, et al. Crack precursor size for natural rubber inferred from relaxing and non-relaxing fatigue experiments. Int J Fatigue 2015;80:50–7.
Trabelsi S, Albouy P-A, Rault J. Effective local deformation in stretched filled rubber macromolecules. Macromolecules 2003;36(24):9093–9.
Beurrot-Borgarino S, Huneau B, Verron E, Rublon P. Strain-induced crystallization of carbon black-filled natural rubber during fatigue measured by in situ synchrotron X-ray diffraction. Int J Fatigue 2013;47:1–7. Candau N, Chazeau L, Chenal J, Gauthier C, Munch E. Compared abilities of
filled and unfilled natural rubbers to crystallize in a large strain rate domain. Compos Sci Technol 2015;108:9–15.
 Rublon P. Etude expérimentale multi-échelle de la propagation de fissure de fatigue dans le caoutchouc naturel. PhD Thesis: Ecole Centrale de Nantes; 2013 [in French].
Candau N, Laghmach R, Chazeau L, Chenal J, Gauthier C, Biben T, et al. Influence of strain rate and temperature on the onset of strain induced crystallization in natural rubber. Eur Polym J 2015;64:244–52.
Andre N, Cailletaud G, Piques R. Haigh diagram for fatigue crack initiation prediction of natural rubber components. Kautschuk Gummi Kunststoffe 1999;52(2):120–3.
Saintier N, Cailletaud J, Piques P. Multiaxial fatigue life prediction for a natural rubber. Int J Fatigue 2006;28(5–6):530–9.
Saintier N, Cailletaud J, Piques P. Cyclic loadings and crystallization of natural rubber: an explanation of fatigue crack propagation reinforcement under a positive loading ratio. Mater Sci Eng A 2011;528:1078–86.
Rublon P, Huneau B, Verron E, Saintier N, Beurrot S, Leygue A, et al. Multiaxial deformation and strain-induced crystallization around a fatigue crack in natural rubber. Eng Fract Mech 2014;123:59–69.
Candau N, Laghmach R, Chazeau L, Chenal J, Gauthier C, Biben T, et al. Strain induced crystallization and melting of natural rubber during dynamic cycles. Phys Chem Chem Phys 2015;17(23):15331–8.
Young D. Fatigue crack propagation in elastomer compounds: effects of strain rate, temperature, strain level and oxidation. Rubber Chem Technol 1986;59:809–25.
Albouy PA, Marchal J, Rault J. Chain orientation in natural rubber, Part I: The inverse yielding effect. Eur Phys J. E, Soft Matter 2005;17(3):247–59. Hamed GR, Kim HJ. Cut growth in vulcanizates of natural rubber,
cis-polybutadiene, and a 50/50 blend: Part II. Cracking patterns in the strained state. Rubber Chem Technol 1999;72(5):895–909.
Huneau B, Masquelier I, Marco Y, Le Saux V, Noizet S, Schiel C, et al. Fatigue crack initiation in a carbon black-filled natural rubber. Rubber Chem Technol 2016;89(1):126–41.